Presentation on theme: "Self Compacting Concrete (SCC)"— Presentation transcript:
1 Self Compacting Concrete (SCC) Prepared By Ravi Kumar
2 Contents Introduction Problems with conventional concrete Benefits of SCCMix design principlesConstituent materialsProperties of fresh SCCTestsApplicationReferences
3 IntroductionFresh concrete that can flow around reinforcement and consolidate within formwork under its own weight that exhibits no defects due to segregation or bleeding.The guiding principle for this type of concrete is that the sedimentation velocity of a particle is inversely proportional to the viscosity of the floating medium in which the particle exists.Source: https://wwwbuildipedia.com
4 Problems with Conventional Concrete Requirement of skilled worker for compaction in conventional concreteDifficult to use mechanical compaction forUnderwater concretingCast in-situ pile foundationColumns with congested reinforcement
5 Benefits of SCC Faster construction Reduction in site manpower Safer working environmentImproved aestheticsEasier placingImproved durability
6 Requirements for Self-compacting concrete Filling abilityPassing abilitySegregation resistance
7 Mix design principlesThe flowability and viscosity of the paste is adjusted by proportioning the cement and additives water to powder ratio and then by adding super plasticizers and VMA .The paste is the vehicle for the transport of the aggregate, therefore the volume of the paste must be greater than the void volume in the aggregate.In order to control temperature rise and thermal shrinkage cracking as well as strength, the fine powder should be added to keep the cement content at an acceptable level. e.g. fly ash, mineral filler, silica fume etc.
8 Contd. SCC should have Low coarse aggregate content Increased paste contentLow water powder ratioIncreased super plasticizer dosageViscosity modifying agents
9 Flow Chart for achieving self compactibility Reduction of water to binder ratioLimitation of coarse aggregate content & maximum sizeAddition of mineral admixtureUsage of Super plasticizer & VMAHigh segregation resistance of mortar & concreteHigh Deformability of mortar & concreteSelf compactibility
10 Typical mix proportion values ConstituentTypical range by volume(liter/m3)PowderWaterCoarse aggregatewater to powder ratioFine aggregate48-55% of total aggregate weight
11 Materials SelectionLimits on the amount of marginally unsuitable aggregate.Choice of HRWRChoice of VMAInteraction & compatibility between cement, HRWR, VMA
12 AggregateIt is observed from these studies that self-compactability is achievable at lower cement (or fines) content when rounded aggregates are used, as compared to angular aggregates.Rounded aggregates would provide a better flowability and less blocking potential for a given water-to-powder ratio, compared to angular and semi-rounded aggregates.To eliminate the poor gradation problem in aggregates, filler materials are used.
13 Chemical AdmixturesHRWRA helps in achieving excellent flow at low water contents and VMA reduces bleeding and improves the stability of the concrete mixture.HRWRAs that work on the principle of steric hindrance require a lower dosage compared to those based on electrostatic repulsion.Acrylic copolymers (AC) and polycarboxylate ethers (PCE) are effective at lower dosages compared to sulfonated condensates of melamine (SMF) or naphthalene (SNF) formaldehyde.
14 Mineral AdmixtureFly ash: It reduces free drying shrinkage and restrains the shrinkage cracking width.Silica fume: it gives good cohesion, improved resistance to segregation. Silica fume is also very effective in reducing or eliminating bleeding.Mineral fillers: The particle size distribution shape and water absorption of mineral fillers may affect the water demand or sensitivity. CaCO3 based minerals fillers (<0.125mm size) are widely used and can give excellent rheological properties and performance.
15 Fresh Properties of SCC Filling AbilitySlump flow test, T50 cm slump flow test, V-Funnel testPassing abilityJ-ring test, U-box, L-boxSegregation potentialSettlement column Test, Sieve stability test, Penetration test
16 Slump Flow TestIt is done to access the horizontal flow of concrete in the absence of obstruction.It gives good assessment of filling ability.Slump cone of 300 mm height, 100 mm upper diameter and 200 mm bottom diameter.The diameter of spread should be lie between 650 mm to 800 mm.The higher the flow value, greater its ability to fill formwork .
18 J-Ring Test It determines the passing ability of SCC. It consist of ring of reinforcement bars that will fit around the slump cone.Slump cone is fitted with concrete and lifted up as in slump cone test.The acceptable difference in height between inside and outside should be between 0 and 10 mm.
20 CuringTop surface dry quickly because of the increased quantity of paste, the low water/fines ratio and the lack of bleed water at the surface.To avoid this Initial curing should therefore commence as soon as practicable after placing and finishing in order to minimize the risk of surface crusting and shrinkage cracks caused by early age moisture evaporation.
21 Complexities involved in SCC Higher paste volume results in greater shrinkage and creep.Higher strength achievement leads to reduces the workability to unacceptable levelLateral Formwork pressureLimit of flow distance of the concrete
22 ApplicationTwo anchorages of Akashi-Kaikyo (Straits) Bridge, Japan. The volume of the cast concrete in the two anchorages amounted to 290,000 m3The highest use of SCC in India was done at Delhi metro project. About m3 of SCC has been Used.At Kaiga nuclear power plant, SCC of Characteristic strength 30 MPa was used.
23 Contd.The Burj Khalifa is the tallest building in the world. SCC was used throughout the building and was pumped 166 stories above the ground.The Trump Tower in Chicago, Illinois was a major user of SCC. It is a 92-story reinforced concrete project that required 3500 m3of SCC to be cast-in- place continuously for 22 hours to construct the mat foundation that supports the finished structure. The mix had a 7-day compressive strength of 68 MPa and a 28-day strength of 82 MPa . This single pour is the largest ever recorded to date in North America using SCC
24 ConclusionWe can reduce the in-place cost and maker a safer working environment for the workers.SCC can be effectively placed in most congested areas and also where normal methods of vibration are not possible.Further research are required to interpret influence on the hardened properties of SCC more precisely.The cost of SCC is % higher than the conventional concrete.
25 ReferencesOkamura et al. “Self-compacting concrete,” Journal of Advanced Concrete Technology, vol. 1, no. 1, pp. 5–15,2003SK Singh “Self Compacting Concrete - A Paradigm Shift”, Journal of New Building Materials & Construction World, Vol. 15, No. 3, pp ,September , 2009.The European Guidelines for Self Compacting Concrete, May 2005Eric P. Koehler et al. Aggregate in Self Consolidating Concrete, ICAR Project 108, March 2007KHALEEL, O.R. et al. The Effect of Coarse Aggregate on Fresh and Hardened Properties of Self-Compacting Concrete (SCC), Elsevier, pp , 2011
26 Contd.Filho et al. Hardened properties of self-compacting concrete — A statistical approach, Elsevier, Construction and Building Materials, pp , 2010Schindler, K Anton et al. Properties of self-consolidating concrete for precast members, ACI Materials Journal, V. 104, No. 1, 2007Specification and Guidelines for Self-Compacting Concrete, EFNARC, 2002Ouchi et al. APPLICATIONS OF SELF-COMPACTING CONCRETE IN JAPAN, EUROPE AND THE UNITED STATES, ISHPC, 2003R. Loser, A. Leemann, Shrinkage and restrained shrinkage cracking of self- compacting concrete compared to conventionally vibrated concrete, Materials and Structures, 2008